CHARACTERIZING MECHANICAL PROPERTIES OF GRAPHITE USING MOLECULAR DYNAMICS SIMULATION


 Hubert Charles
 10 months ago
 Views:
Transcription
1 CHARACTERIZING MECHANICAL PROPERTIES OF GRAPHITE USING MOLECULAR DYNAMICS SIMULATION JiaLin Tsai and JieFeng Tu Department of Mechanical Engineering, National Chiao Tung University 1001 University Road, Hsinchu, Taiwan 300 SUMMARY When the graphite was employed as reinforcement in composites, it may aggregate in the form of graphite flakes (containing several graphite nanoplatelets) or exfoliate into single graphite layers (graphene). Results obtained from molecular dynamics (MD) simulation indicated that the graphene exhibit higher moduli than the graphic flakes. Keywords: MD simulation, Graphite, Material properties 1. INTRODUCTION With the characteristics of high strength and stiffness, the graphite has been used as reinforcements in composite materials [1]. The natural graphite is constructed by numbers of graphene layers with interlayer spacing of around 3.4Å. Through chemical oxidation in the environment of sulfuric and nitric acid, the acid intercalant can be intercalated into the graphite galleries to form an intercalated graphite compound. Subsequently, by applying rapid heating because of the vaporization of the acid intercalant in the graphite galleries, the interacted graphite was significantly expanded along the thickness direction and converted into the expanded graphite (EG). After a mechanical mixer together with sonication process, the expanded graphite was dispersed and exfoliated into the polymer matrix to form graphitereinforced nanocomposites. The synthesizing process for manufacturing the nanocomposites was discussed in detail in the literatures [, 3]. However, the stacked graphene structures (so called graphite flakes) are commonly observed in TEM micrographs and XRD examination [4], and it is a challenging task to fully exfoliate the aggregated graphene sheets. In fact, graphite flakes together with graphene layers are commonly observed in graphite nanocomposites and it is important to clarify if the two atomistic configurations of the graphite, i.e., graphite flakes and single graphene layer, would have the same mechanical properties. Moreover, in order to accurately characterize the mechanical properties of the graphitereinforced nanocomposites, an exploration of the fundamental properties of the graphite associated with different microstructures is required. Cho et al. [5] performed a molecular structural analysis to calculate the graphite s elastic constants. The inplane properties of graphite were derived by considering the geometric deformation of a single graphene sheet subjected to inplane loading. However, for the outofplane properties, they modeled the graphic as graphic flake
2 with multi graphene layers, the nonbonded atomistic interactions of which were described using LennardJones potential function. By using MD simulation, Bao et al. [6] investigated the variations of Young s modulus of graphite, which contains different numbers of graphene layers (one to five layers). Results indicated that there is no considerable difference in Young s modulus between the single layer of graphene and graphite flakes with five layers of graphene. Reddy et al. [7] modeled the elastic properties of a finitesized graphene sheet using continuum mechanics approach based on Brenner s potential [8]. The computed elastic constants of the graphene sheet are found to follow the orthotropic material behaviors. In light of the forgoing, most studies characterize the elastic properties of the graphite based on the behavior of a single graphene sheet; the mutual influences of the adjacent graphene layers on the mechanical responses in the graphite flakes are rarely taken into account. As previously mentioned, both the graphene layer and the graphite flakes were commonly found in the nanocomposites, so it is not adequate to utilize the properties of the graphene sheet instead of the graphite flakes in the modeling of graphitereinforced nanocomposites. In this study, the mechanical properties of the graphite flakes and the graphene were systematically characterized using MD simulation. Both bonded and nonbonded interactions were accounted for in the description of the atomistic graphite structures. By applying uniaxial tensile loading on the atomistic graphite structures, the Young s modulus and Poisson s ratio were determined from the strain field in the deformed configuration. In the same manner, the shear modulus was predicted from the shear deformation associated with the applied shear stress. The properties of the single graphene layer were then compared to those of the graphite flakes with multilayers of graphene.. MOLECULAR DYNAMICS SIMULATION.1 Construction of atomistic structures of graphite Graphite structure is constructed by the carbon layers where the carbon atoms are arranged in a hexagonal pattern. The interatomistic distance between the adjacent carbon atoms is 1.4Å, and the associated atomistic interaction is covalently bonded by sp hybridized electrons, the bond angle of which is 10 degree to each other. In naturally occurring or high quality synthetic graphite, the carbon layers are attacked along the thickness direction in AB type sequence with interlayer spacing of approximately 3.4Å. Hereafter, the graphite with several carbon layers lumped together is referred to as graphite flakes. Because the adjacent carbon layers are held together by the weak van der Waals force, after proper processing [, 3], the stacked carbon layers can be dispersed and separated into a single layer that is usually called graphene sheet or graphene layer. In order to investigate the mechanical properties of the graphite flakes and the graphene layer, the atomistic structures have to be constructed in conjunction with the appropriately specified atomistic interaction. In the description of graphite structure, two kinds of atomistic interactions are normally taken in account; one is bonded interaction, such as the covalent bond, and the other is the nonbonded interaction, i.e., van der Waals and electrostatic forces. Among the atomistic interactions, the covalent
3 bond between two neighboring carbon atoms that provides the building block of the primary structure of the graphite may play an essential role in the mechanical responses. Such bonded interaction can be described using the potential energy that consists of bond stretching, bond angle bending, torsion, and inversion [9]. Therefore, the total potential energy of the graphite contributed from the covalent bond is given as U graphite = Ur + Uθ + Uφ + Uω (1) where U r is a bond stretching potential; U θ is a bond angle bending potential; U φ is a dihedral angle torsional potential; and U ω is an inversion potential. For graphite structures under inplane deformation, the atomistic interaction is mainly governed by the bond stretching and bond angle bending therefore, the dihedral torsion and inversion potentials that are related to the outofplane deformation were disregarded in the modeling. The explicit form for the bond stretching and bond angle bending can be approximated in terms of elastic springs as [10] U r 1 = k ( ) r r r0 () 1 U ( ) θ = kθ θ θ 0 (3) where k r and k θ are the bond stretching force constant and angle bending force kcal kcal constant, respectively. The constants k = r mole nm and kθ = 16 mole rad selected from AMBER force field for carboncarbon atomicinteraction [11] was employed in our molecular simulation. The parameters r 0 and θ 0 represent bond length and bond angle in equilibrium position, which are assumed to be 1.4 Å and 10 o, respectively, for the graphite atomistic structures. In addition to the bonded interaction, the nonbonded interaction between the carbon atoms was regarded as the van der Waals force, which can be characterized using the LennardJones (LJ) potential as 1 6 r0 r0 U vdw = 4u (4) rij rij
4 where r ij is the distance between the nonbonded pair of atoms. For the hexagonal graphite, the parameters u = kcal/mole and r 0 = 3.40 Å suggested in the literature [1] were adopted in the modeling. Moreover, the cutoff distance for the van der Waals force is assigned to be 10Ǻ, which means that beyond this distance, there are no more van der Waals interactions taking place. In order to model the material properties of graphite flakes and the graphene sheet, the simulation box suitable for representing the corresponding atomistic structures has to be established. Fig. 1 shows the schematic of the simulation box for graphite flakes and the graphene sheet as well. A periodic boundary condition was implemented on all surfaces to demonstrate the infinite graphite structures. It is noted in the graphene sheet that the dimension of the simulation box in the thickness direction is set to be large enough that the van der Waals interaction between the neighboring layers can not be attained. This especial design of the simulation box is intended to simulate the exfoliated graphene sheets. The NPT ensemble [13] with temperature at 0K and pressure equal to 0 was conducted to achieve the stressfree configuration. The MD simulation was carried out under the DLPOLY package originally developed by Daresbury Laboratory [14] in conjunction with the homemade subroutine for postprocessing.. Characterizing the Young s modulus and Poisson s ratio of the graphite The methodology developed to evaluate the mechanical properties of the atomistic structures was motivated from the technique commonly used in the continuum solid. For continuum solids, the Young s modulus and Poisson s ratio are measured from the simple tension test. The same concept was extended and applied to the atomistic structures by means of a modified NPT ensemble in MD simulation with the characteristics of varying a simulation box in shape and size [15]. In other words, axial stresses can be implemented on both sides of the simulation box with other faces being traction free as shown in Fig.. Again, after the energy minimization process, the equilibrated graphite atomistic structure under axial loading was obtained, and the Young s modulus and Poisson s ratio was defined in the continuum manner as E σ = (5) ε 1 ε ν 1 = (6) ε1 where ε 1 is the strain component measured in the loading direction, and ε is the strain component measured in the lateral direction. As is noted in equation (5), σ should be the stress directly acting on the graphite structure. However, for the case of graphene sheet as shown in Fig. (a), because the dimension of the graphene sheet in thickness direction is not compatible to the size of the simulation box, the stress in the graphene
5 sheet has to be converted from the stress acting on the simulation box, σ box, in terms of the geometric parameters as σ box h σ = (7) t where h is the height of the simulation box, and t is the thickness of the graphene sheet, which is equal to 3.4Å. The Young s modulus and Poisson s ratio obtained from MD simulation for the graphite flakes and graphene sheet are presented, respectively, in Table Characterization of Shear modulus G 1 By following the same technique used in the early section, the shear modulus of the atomistic structure can be evaluated via the application of inplane shear stress on the simulation box as shown in Fig. 3. This process is accomplished by conducting the modified NPT ensemble in MD simulation. After the energy minimization process, the deformed configuration of the simulation box was calculated from which the shear strain associated with the applied shear stress was determined. If the deformation is small, the shear modulus of the graphite can be defined based on the theory of linear elasticity as τ G = (8) γ where τ is the applied shear stress, and γ is the corresponding shear strain determined from MD simulation. The shear moduli calculated with equation (8) for the graphite flakes and graphene sheet are also listed in Table RESULTS AND DISCUSSION Results presented in Table 1 indicate that the single graphene sheet demonstrates higher Young s modulus and shear modulus than the graphite flakes. Thus, it was suggested that to achieve better mechanical properties of nanocomposites, the aggregated graphite flakes need to be exfoliated in the form of graphene sheets and uniformly dispersed into the matrix systems. Moreover, according to the relationship between Young s modulus, shear modulus, and Poisson s ratio, it was found that both graphite flakes and graphene demonstrate isotropic inplane properties. This isotropic property could be attributed to the hexagonal array of the carbon atoms. For the purposes of comparing, the calculated material properties of the graphite are listed together with other published predictions in Table. It was revealed that the moduli obtained from the current model are a little less than those listed in the literature
6 although the discrepancy is not much. This difference could be resulting from the different potential functions employed in the modeling of the atomistic interaction of the carbon atoms. On the other hand, it should be indicated that most of the published values are calculated based on the graphene sheet except the one addressed by Bao et al. [6] who investigated the Young s modulus of graphite with numbers of graphene layers (from one layer up to five layers). In their investigation, there is no significant difference in Young s modulus between the single graphene layer and the graphite flake with fivelayer graphene. It is possible that the dissimilarity may not be considerable just by comparing the single layer graphene with the fivelayer graphene. On the contrary, our prediction considers the periodic boundary condition in the thickness direction and would be close to the behavior of the graphite flakes with numbers of graphene layers. This is the reason why in our simulation, the graphic flacks would exhibit different material properties from the single graphene sheet. In addition, for the sake of comparison, the experimental values for the graphite structures provided by Blakslee et al. [16] were added in Table. It shows that the values predicted based on the graphene sheet model have a better agreement with the experimental data. 4. CONCLUSION The inplane properties of graphene sheet and the graphite flakes were investigated using MD simulation by performing simple loading on the atomistic structures. Because of the hexagonal array of the carbon atoms, the inplane shear modulus, Young s modulus, and Poisson s ratio of the graphite flakes and graphene sheet satisfy the isotropic properties. A comparison of inplane properties of the graphene sheet and graphite flakes reveals that the single graphene sheet exhibits higher modulus than the graphite flakes; therefore, the exfoliation of the graphite flakes into graphene layers is essential in order to have better mechanical properties of graphitereinforced nanocomposites. ACKNOWLEDGMENTS This research was supported by the National Science Council, Taiwan, under the contract No. NSC E to National Chiao Tung University.
7 Table 1 Comparison of inplane elastic constants of graphite flakes and graphene E (TPa) ν G 1 (TPa) Graphene Graphite flakes Table Comparison of the predicted values with others listed in the literatures Graphene Graphite flakes Cho et al [5] Bao et al [6] Reddy et al [7] Blakslee et al [] E (TPa) ν G 1 (TPa) Å 3.4 Å A B A B A B A B 3.4 Å 7. Å (a) Fig. 1. Schematic of atomistic model in the MD simulation for (a) graphene sheet and (b) graphite flakes (b)
8 x 3 x x 1 (a) (b) Fig.. Axial stress applied in (a) graphene sheet and (b) graphite flakes Fig. 3. Inplane shear stress applied in (a) graphene sheet and (b) graphite flakes References [1] Fukushima H, Drzal LT. Graphite Nanoplatelets as Reinforcements for Polymers: Structural and Electrical Properties. In: Proceedings of the American Society for Composites, The 17 th technical conference, 13 October; 00. [] Li J, Kim JK, Sham ML. Conductive Graphite Nanoplatelet/Epoxy Nanocomposites: Effect of Exfoliation and UV/Ozone Treatment of graphite. Scr Mater 005;53: [3] Fukushima H, Drzal LT, Rook BP, Rich MJ. Thermal Conductivity of Exfoliated Graphite Nanocomposites. J Therm Anal Calorim 006;85(1): [4] Yasmin A, Luo JJ, Daniel IM. Processing of Expanded Graphite Reinforced Polymer Nanocomposites. Compos Sci Technol 006;66:1189.
9 [5] Cho J, Luo JJ, Daniel IM. Mechanical Characterization of Graphite/Epoxy Nanocomposites by Multiscale Analysis. Compos Sci Technol 007;67: [6] Bao WX, Zhu CC, Cui WZ. Simulation of Young s Modulus of Singlewalled Carbon Nanotubes by Molecular Dynamics. Physica B 004;35: [7] Reddy CD, Rajendran S, Liew KM. Equilibrium Configuration and Continuum Elastic Properties of Finite Sized Graphene. Nanotechnology 006;17: [8] Brenner DW. Empirical Potential for Hydrocarbons for Use Simulating the Chemical Vapor Deposition of Diamond Films. Phys Rev B 1990;4(15): [9] Rappe AK, Casewit CJ. Molecular Mechanics Across Chemistry. Sausalito, CA: University Science Books; [10] Li C, Chou TW. A Structural Mechanics Approach for the Analysis of Carbon Nanotubes. Int J Solids Struct 003;40(10): [11] Cornell WD, Cieplak P, Bayly CI, Gould IR, Merz KM, Jr, Ferguson DM, Spellmeyer DC, Fox T, Caldwell JW, Kollman PA. A Second Generation Force Field for the Simulation of Proteins, Nucleic Acids, and Organic Molecules. J Am Chem Soc 1995;117(19): [1] Battezzatti L, Pisani C, Ricca F. Equilibrium conformation and surface motion of hydrocarbon moleculars physisorbed on graphite. J Chem Soc 1975;71: [13] Allen MP, Tildesley DJ. Computer Simulation of Liquids. Oxford: Clarendon Press; [14] Smith W, Forester TR. The DL_POLY User Manual, version.13. England, Warrington WA4 4AD: Daresbury, Daresbury Laboratory, CCLRC; 001. [15] Melchionna S, Ciccotti G, Holian BL. Hoover NPT Dynamics for Systems Varying in Shape and Size. Mol Phys 1993;78(3): [16] Blakslee OL, Proctor DG, Seldin EJ, Spence GB, Weng T. Elastic Constants of CompressionAnnealed Pyrolytic Graphite. J Appl Phys 1970;41:
Nonlinear Mechanics of Monolayer Graphene Rui Huang
Nonlinear Mechanics of Monolayer Graphene Rui Huang Center for Mechanics of Solids, Structures and Materials Department of Aerospace Engineering and Engineering Mechanics The University of Texas at Austin
More informationIntroduction to molecular dynamics
1 Introduction to molecular dynamics Yves Lansac Université François Rabelais, Tours, France Visiting MSE, GIST for the summer Molecular Simulation 2 Molecular simulation is a computational experiment.
More informationWhy Proteins Fold? (Parts of this presentation are based on work of Ashok Kolaskar) CS490B: Introduction to Bioinformatics Mar.
Why Proteins Fold? (Parts of this presentation are based on work of Ashok Kolaskar) CS490B: Introduction to Bioinformatics Mar. 25, 2002 Molecular Dynamics: Introduction At physiological conditions, the
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationNonlocal material properties of single walled carbon nanotubes
Nonlocal material properties of single walled carbon nanotubes J. V. Araújo dos Santos * and C. M. Mota Soares IDMEC, Instituto Superior Técnico, Universidade Técnica de Lisboa, Portugal Av. Rovisco Pais,
More informationIntensity (a.u.) Intensity (a.u.) Raman Shift (cm 1 ) Oxygen plasma. 6 cm. 9 cm. 1mm. Singlelayer graphene sheet. 10mm. 14 cm
Intensity (a.u.) Intensity (a.u.) a Oxygen plasma b 6 cm 1mm 10mm Singlelayer graphene sheet 14 cm 9 cm Flipped Si/SiO 2 Patterned chip Plasmacleaned glass slides c d After 1 sec normal Oxygen plasma
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationNew Sixsite Acetonitrile Model for Simulations of Liquid Acetonitrile and its Aqueous Mixtures
New Sixsite Acetonitrile Model for Simulations of Liquid Acetonitrile and its Aqueous Mixtures ALEXEI M. NIKITIN, 1,2 ALEXANDER P. LYUBARTSEV 2 1 Engelhardt Institute of Molecular Biology Russian Academy
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationInternal lattice relaxation of singlelayer graphene under inplane deformation. Jun Zhou and Rui Huang
Internal lattice relaxation of singlelayer graphene under inplane deformation Jun Zhou and Rui Huang Department of Aerospace Engineering and Engineering Mechanics, University of Texas, Austin, TX 7871
More informationDefense Technical Information Center Compilation Part Notice
UNCLASSIFIED Defense Technical Information Center Compilation Part Notice ADP012151 TITLE: Chemical Bonding of Polymer on Carbon Nanotube DISTRIBUTION: Approved for public release, distribution unlimited
More informationA Molecular Dynamics Simulation of a Homogeneous OrganicInorganic Hybrid Silica Membrane
A Molecular Dynamics Simulation of a Homogeneous OrganicInorganic Hybrid Silica Membrane Supplementary Information: Simulation Procedure and Physical Property Analysis Simulation Procedure The molecular
More informationBrazilian Journal of Physics ISSN: Sociedade Brasileira de Física Brasil
Brazilian Journal of Physics ISSN: 01039733 luizno.bjp@gmail.com Sociedade Brasileira de Física Brasil Rouhi, S.; Alizadeh, Y.; Ansari, R. On the Wrapping of Polyglycolide, Poly(Ethylene Oxide), and Polyketone
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationElastic Deformation Mechanics of Cellulose Nanocrystals
Elastic Deformation Mechanics of Cellulose Nanocrystals Xiawa Wu 1, Ryan Wagner 1,2, Arvind Raman 1,2, Robert Moon 2,3,4, Ashlie Martini 1 1 School of Mechanical Engineering, Purdue University 2 Birck
More informationGraphenereinforced elastomers for demanding environments
Graphenereinforced elastomers for demanding environments Robert J Young, Ian A. Kinloch, Dimitrios G. Papageorgiou, J. Robert Innes and Suhao Li School of Materials and National Graphene Institute The
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationMolecular modeling of EPON862/graphite composites: Interfacial characteristics for multiple crosslink densities
Molecular modeling of EPON862/graphite composites: Interfacial characteristics for multiple crosslink densities C.M. Hadden 1, B.D. Jensen 1, A. Bandyopadhyay 1, G.M. Odegard 1 *, A. Koo 2, R. Liang 2,
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationarxiv: v1 [condmat.statmech] 6 Jan 2014
arxiv:1401.1181v1 [condmat.statmech] 6 Jan 2014 Determination of Forces from a Potential in Molecular Dynamics (note) Bernard Monasse MinesParisTech, Cemef bernard.monasse@minesparistech.fr January
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationInfluence of temperature and voltage on electrochemical reduction of graphene oxide
Bull. Mater. Sci., Vol. 37, No. 3, May 2014, pp. 629 634. Indian Academy of Sciences. Influence of temperature and voltage on electrochemical reduction of graphene oxide XIUQIANG LI, DONG ZHANG*, PEIYING
More informationNumerical Modeling of Delamination Resistance Improvement Through The Use of CNTReinforced Bonding Layers
21 st International Conference on Composite Materials Xi an, 2025 th August 2017 Numerical Modeling of Delamination Resistance Improvement Through The Use of CNTReinforced Bonding Layers Yassine ElAssami
More information*MAT_PAPER  a new orthotropic elastoplastic model for paper materials
*MAT_PAPER  a new orthotropic elastoplastic model for paper materials Jesper Karlsson, Dynamore Nordic Mikael Schill, Dynamore Nordic Johan Tryding, Tetra Pak *MAT_PAPER (*MAT_274) A new orthotropic elastoplastic
More informationRESEARCH PROJECT NO. 26
RESEARCH PROJECT NO. 26 DETERMINATION OF POISSON'S RATIO IN AD1 TESTING BY UNIVERSITY OF MICHIGAN REPORT PREPARED BY BELA V. KOVACS and JOHN R. KEOUGH \ MEMBER / / DUCTILE IRON \ SOCIETY Issued by the
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationThe Young s Modulus of SingleWalled Carbon Nanotubes
The Young s Modulus of SingleWalled Carbon Nanotubes Douglas Vodnik Faculty Advisor: Dr. Kevin Crosby Department of Physics, Carthage College, Kenosha, WI Abstract A new numerical method for calculating
More informationDelamination in the scoring and folding of paperboard
PEERREVIEWED CONVERTING Delamination in the scoring and folding of paperboard DOEUNG D. CHOI, SERGIY A. LAVRYKOV, and BANDARU V. RAMARAO ABSTRACT: Delamination between layers occurs during the creasing
More informationComputer Simulations of Carbon Nanostructures under Pressure
Fullerenes, Nanotubes, and Carbon Nanostructures, 13: 13 20, 2005 Copyright # Taylor & Francis, Inc. ISSN 1536383X print/15364046 online DOI: 10.1081/FST200039164 Computer Simulations of Carbon Nanostructures
More informationMD simulation of methane in nanochannels
MD simulation of methane in nanochannels COCIM, Arica, Chile M. Horsch, M. Heitzig, and J. Vrabec University of Stuttgart November 6, 2008 Scope and structure Molecular model for graphite and the fluidwall
More informationCE 530 Molecular Simulation
1 CE 530 Molecular Simulation Lecture 1 David A. Kofke Department of Chemical Engineering SUNY Buffalo kofke@eng.buffalo.edu 2 Time/s MultiScale Modeling Based on SDSC Blue Horizon (SP3) 1.728 Tflops
More informationApplication to modeling brittle materials
1.01, 3.01, 10.333,.00 Introduction to Modeling and Simulation Spring 011 Part I Continuum and particle methods Application to modeling brittle materials Lecture 7 Markus J. Buehler Laboratory for Atomistic
More informationImperfect Gases. NC State University
Chemistry 431 Lecture 3 Imperfect Gases NC State University The Compression Factor One way to represent the relationship between ideal and real gases is to plot the deviation from ideality as the gas is
More informationTEMPERATURE DEPENDENCE OF THE TENSILE PROPERTIES OF SINGLE WALLED CARBON NANOTUBES: O(N) TIGHT BINDING MD SIMULATION GÜLAY DERELİ *, BANU SÜNGÜ
TEMPERATURE DEPENDENCE OF THE TENSILE PROPERTIES OF SINGLE WALLED CARBON NANOTUBES: O(N) TIGHT BINDING MD SIMULATION GÜLAY DERELİ *, BANU SÜNGÜ Department of Physics, Yildiz Technical University, 34210
More informationMultiscale modeling of heat conduction in graphene laminates
Multiscale modeling of heat conduction in graphene laminates Bohayra Mortazavi * and Timon Rabczuk Institute of Structural Mechanics, BauhausUniversität Weimar, Marienstr. 15, D99423 Weimar, Germany
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationFINITE ELEMENT APPROACH TO SIMULATE CNTREINFORCED CALCIUMSILICATEHYDRATE (CSH) COMPOSITE
Proceedings of the 7th International Conference on Mechanics and Materials in Design Albufeira/Portugal 1115 June 2017. Editors J.F. Silva Gomes and S.A. Meguid. Publ. INEGI/FEUP (2017) PAPER REF: 6782
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationA General Equation for Fitting Contact Area and Friction vs Load Measurements
Journal of Colloid and Interface Science 211, 395 400 (1999) Article ID jcis.1998.6027, available online at http://www.idealibrary.com on A General Equation for Fitting Contact Area and Friction vs Load
More informationAnalysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements
Acta Mech. Sin. (2016) 32(2):295 300 DOI 10.1007/s1040901505342 RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1
More informationComputational Chemistry. An Introduction to Molecular Dynamic Simulations
Computational Chemistry An Introduction to Molecular Dynamic Simulations Computational chemistry simulates chemical structures and reactions numerically, based in full or in part on the fundamental laws
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationMultiscale Materials Modeling
Multiscale Materials Modeling Lecture 02 Capabilities of Classical Molecular Simulation These notes created by David Keffer, University of Tennessee, Knoxville, 2009. Outline Capabilities of Classical
More informationCombined Stresses and Mohr s Circle. General Case of Combined Stresses. General Case of Combined Stresses con t. Twodimensional stress condition
Combined Stresses and Mohr s Circle Material in this lecture was taken from chapter 4 of General Case of Combined Stresses Twodimensional stress condition General Case of Combined Stresses con t The normal
More informationCOMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS. Abstract. Introduction
COMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS HsiangChuan Tsai, National Taiwan University of Science and Technology, Taipei, Taiwan James M. Kelly, University of California,
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationMolecular Mechanics / ReaxFF
Molecular Dynamics simulations Lecture 09: Molecular Mechanics / ReaxFF Dr. Olli Pakarinen University of Helsinki Fall 2012 Lecture notes based on notes by Dr. Jani Kotakoski, 2010 CONTENTS Molecular mechanics
More informationBending Analysis of a Cantilever Nanobeam With End Forces by Laplace Transform
International Journal of Engineering & Applied Sciences (IJEAS) Vol.9, Issue (Special Issue: Composite Structures) (07) 03 http://.doi.org/0.407/ijeas.34635 Int J Eng Appl Sci 9() (07) 03 Bending Analysis
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationInteractioninduced depolarized light scattering spectra of exohedral complexes of Ne and Ar with fullerenes and nanotubes
Materials SciencePoland, Vol. 3, No., 005 Interactioninduced depolarized light scattering spectra of exohedral complexes of Ne and Ar with fullerenes and nanotubes Z. DENDZIK *, M. KOŚMIDER, A. DAWID,
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationMOLECULAR MODELLING OF STRESSES AND DEFORMATIONS IN NANOSTRUCTURED MATERIALS
Int. J. Appl. Math. Comput. Sci., 2004, Vol. 14, No. 4, 541 548 MOLECULAR MODELLING OF STRESSES AND DEFORMATIONS IN NANOSTRUCTURED MATERIALS GWIDON SZEFER Institute of Structural Mechanics, AGH University
More informationNonlinear Viscoelastic Behaviour of Rubber Composites
Nonlinear Viscoelastic Behaviour of Rubber Composites Sabu Thomas Centre for Nanoscience and Nanotechnology, Mahatma Gandhi University, Kottayam India 1 Polymer Nanocomposites Spheres (0D) TiO 2, SiO 2
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More informationTimedependence of key Hbond/electrostatic interaction distances in the sirna5hago2 complexes... Page S14
Supporting Information Probing the Binding Interactions between Chemically Modified sirnas and Human Argonaute 2 Using Microsecond Molecular Dynamics Simulations S. Harikrishna* and P. I. Pradeepkumar*
More informationChapter 11 Molecular Mechanics
Chapter 11 Molecular Mechanics Molecular Mechanics uses an analytical, differentiable, and relatively simple potential energy function, (R), for describing the interactions between a set of atoms specified
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationThe Relationship between the Applied Torque and Stresses in PostTension Structures
ECNDT 6  Poster 218 The Relationship between the Applied Torque and Stresses in PostTension Structures Fui Kiew LIEW, Sinin HAMDAN * and Mohd. Shahril OSMAN, Faculty of Engineering, Universiti Malaysia
More informationA MOLECULAR DYNAMICS SIMULATION OF A BUBBLE NUCLEATION ON SOLID SURFACE
A MOLECULAR DYNAMICS SIMULATION OF A BUBBLE NUCLEATION ON SOLID SURFACE Shigeo Maruyama and Tatsuto Kimura Department of Mechanical Engineering The University of Tokyo 7 Hongo, Bunkyoku, Tokyo 866,
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More informationSolid State Theory Physics 545
olid tate Theory hysics 545 Mechanical properties of materials. Basics. tress and strain. Basic definitions. Normal and hear stresses. Elastic constants. tress tensor. Young modulus. rystal symmetry and
More informationComputational Methods. Chem 561
Computational Methods Chem 561 Lecture Outline 1. Ab initio methods a) HF SCF b) PostHF methods 2. Density Functional Theory 3. Semiempirical methods 4. Molecular Mechanics Computational Chemistry " Computational
More information*MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials
14 th International LSDYNA Users Conference Session: Constitutive Modeling *MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials Jesper Karlsson 1, Mikael Schill 1, Johan Tryding
More informationLinear Cosserat elasticity, conformal curvature and bounded stiffness
1 Linear Cosserat elasticity, conformal curvature and bounded stiffness Patrizio Neff, Jena Jeong Chair of Nonlinear Analysis & Modelling, Uni Dui.Essen Ecole Speciale des Travaux Publics, Cachan, Paris
More informationCurvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment. P. Krulevitch G. C. Johnson
UCRLJC30440 PREPRINT Curvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment P. Krulevitch G. C. Johnson This paper was prepared for submittal to the Materials Research Society Spring
More informationContact, Adhesion and Rupture of Elastic Solids
D. Maugis Contact, Adhesion and Rupture of Elastic Solids With 186 Figures Springer Contents г 1. Elements of Surface Physics 1 1.1 Introduction 1 1.2 Van der Waals Forces Between Molecules 3 1.2.1 The
More informationIntroduction to Nanotechnology Chapter 5 Carbon Nanostructures Lecture 1
Introduction to Nanotechnology Chapter 5 Carbon Nanostructures Lecture 1 ChiiDong Chen Institute of Physics, Academia Sinica chiidong@phys.sinica.edu.tw 02 27896766 Carbon contains 6 electrons: (1s) 2,
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationFondamenti di Chimica Farmaceutica. Computer Chemistry in Drug Research: Introduction
Fondamenti di Chimica Farmaceutica Computer Chemistry in Drug Research: Introduction Introduction Introduction Introduction Computer Chemistry in Drug Design Drug Discovery: Target identification Lead
More informationVibration of quadrilateral embedded multilayered graphene sheets based on nonlocal continuum models using the Galerkin method
Acta Mech Sin 2011 276:967 976 DOI 101007/s1040901105140 RESEARCH PAPER Vibration of quadrilateral embedded multilayered graphene sheets based on nonlocal continuum models using the Galerkin method
More informationSupporting information for Polymer interactions with Reduced Graphene Oxide: Van der Waals binding energies of Benzene on defected Graphene
Supporting information for Polymer interactions with Reduced Graphene Oxide: Van der Waals binding energies of Benzene on defected Graphene Mohamed Hassan, Michael Walter *,,, and Michael Moseler, Freiburg
More informationAn Extended van der Waals Equation of State Based on Molecular Dynamics Simulation
J. Comput. Chem. Jpn., Vol. 8, o. 3, pp. 97 14 (9) c 9 Society of Computer Chemistry, Japan An Extended van der Waals Equation of State Based on Molecular Dynamics Simulation Yosuke KATAOKA* and Yuri YAMADA
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationLecture 7, Foams, 3.054
Lecture 7, Foams, 3.054 Opencell foams StressStrain curve: deformation and failure mechanisms Compression  3 regimes  linear elastic  bending  stress plateau  cell collapse by buckling yielding
More informationRVE Analysis of Light Weight Carbon Nanotubes Embedded Piezoelectric Fibre Composites
Nanoscience and Nanotechnology 2016, 6(1): 1116 DOI: 10.5923/j.nn.20160601.03 RVE Analysis of Light Weight Carbon Nanotubes Embedded Piezoelectric Fibre Composites V. K. Srivastava 1,*, H. Berger 2, U.
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationWater models in classical simulations
Water models in classical simulations Maria Fyta Institut für Computerphysik, Universität Stuttgart Stuttgart, Germany Water transparent, odorless, tasteless and ubiquitous really simple: two H atoms attached
More informationExternal Work. When a force F undergoes a displacement dx in the same direction i as the force, the work done is
Structure Analysis I Chapter 9 Deflection Energy Method External Work Energy Method When a force F undergoes a displacement dx in the same direction i as the force, the work done is du e = F dx If the
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationChapter 12. Insert picture from First page of chapter. Intermolecular Forces and the Physical Properties of Liquids and Solids
Chapter 12 Insert picture from First page of chapter Intermolecular Forces and the Physical Properties of Liquids and Solids Copyright McGrawHill 2009 1 12.1 Intermolecular Forces Intermolecular forces
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More information